- Technical Help
- Find a Supplier
- BSSA Members
- Affiliate Members
Salt spray testing is an accepted method for assessing the suitability of stainless steel parts and fabrications that are likely to encounter chloride environments in service.
For any particular part, tested under laboratory conditions, a difference in performance between say, 430 (1.4016), 304 (1.4301) and 316 (1.4401) types would be expected, but the test outcome is sensitive to the shape of the parts (designed-in crevices), surface finish and the test conditions.
Using specific laboratory salt spray test data to assess if a particular steel grade is suitable for a specific or ‘generic’ environment is therefore not appropriate.
Salt spray testing is covered by the standards such as
ASTM B 117 – Practice for Operating Salt Spray (Fog) Testing Apparatus
Tests durations are not defined, but multiples of 24h are suggested.
BS EN ISO 9227:2017 – Corrosion tests in artificial atmospheres. Salt spray tests which in an earlier version, 2006, superseded BS7479:1991 – Method for Salt Spray Corrosion Tests in Artificial Atmospheres which in turn had superseded BS5466:1977 and was equivalent to ISO 9227.
This standard covers methods in three types of atmospheres: –
The test durations range from 2 to 1008 hours.
The results can be evaluated in a number of ways, (see the original standard), one example of a pass / fail criteria is that there should not be any ‘visible’ staining on parts tested.
The test acceptance criteria can therefore be subjective and need to be clearly defined for any set situation.
Results from one testing laboratory, based on tests done to the ASTM B117 method suggest a 316 type part could be expected to pass a 96 hour test using a 3% salt spray.
Indications are that longer test times would not be expected to give satisfactory results.
In contrast, 304 type parts would not be expected to give satisfactory results in a 3% salt spray, but if the salt solution concentration is reduced to 0.3 %, then it is possible that a 304 type parts may be satisfactory for test times up to 120 hours.
This could also apply to 430 type ferritic or 431 type martensitic stainless steel parts.